### Transport properties of Nb/PdNi bilayers

### C. Cirillo *, S.L. Prischepa

1### , M. Salvato, C. Attanasio

Dipartimento di Fisica ‘E.R. Caianiello’ and INFM, Universita` degli Studi di Salerno, Baronissi (SA) I-84081, Italy

Abstract

The transport properties of superconductor/weak ferromagnet Nb/Pd86Ni14sputtered bilayers have been studied. The critical thickness needed for superconductivity to develop is determined from the dependence of the transition temperature Tcon dNb.

q2005 Elsevier Ltd. All rights reserved.

PACS: 74.45.Cc; 74.78.Fk

1. Introduction

In last years great interest has been devoted to the study of artificial layered structures consisting of superconducting (S) and magnetic layers (F), allowing the investigation of the interplay between two competing orders and revealing a rich variety of phenomena[1–4].

In these systems, the two different materials are coupled by proximity effect. Superconductivity is depressed in S over the coherence length xSand a minimum thickness of the S layer is

necessary to make superconductivity survive. This thickness is called superconducting critical thickness, dcrS.

Superconduc-tivity is also induced in F, but the exchange energy Eex, which

is here the main pair breaking mechanism, depresses superconductivity acting on the spins of the Cooper pairs. Moreover, due to the presence of this field, the superconducting order parameter does not simply decay in the ferromagnetic metal, but it also oscillates over a length scale given, in the dirty limit, by xFZ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃZDF=Eex

p

, the coherence length in F[5]. Here, DFis the diffusion coefficient.

The superconducting transition temperature, TC, is the

simplest parameter which reveals intriguing behaviour typical of the S/F structure, such as a nonmonotonic dependence, both in multilayers and bilayers, as a function of the F layers thickness, dF. However, a clear comparison between the

theoretical predictions [5–8] and the experimental results

[1,9,10] is still controversial, because, at least in systems in

which F is a traditional ferromagnet, the oscillation are predicted and observed in a dF range, where structural and

magnetic properties are also critical[9–11].

For these reasons, we decided to study the Nb/PdNi system, where PdNi is a magnetic alloy, in which the exchange energy, controlled trough the percentage of the magnetic component (Ni) in the metallic high paramagnetic matrix (Pd), is in the meV range[2]. These values lead to a ferromagnetic coherence length of the order of 50–100 A˚ , a thickness accessible to standard deposition techniques. Moreover, PdNi seems to be more intriguing than other weak ferromagnets, such as CuNi, because of the high values of the interface transparency measured in Nb/Pd systems[11,12].

This work is organized as follows: after a brief description of the sample preparation and structural characterization, we will focus on the behaviour of the superconducting transition temperatures of Nb/PdNi bilayers as a function of the Nb thickness.

2. Sample preparation and characterization

Nb/Pd90Ni10bilayers were grown on Si(100) substrates by a

dual source magnetically enhanced dc triode sputtering system with a movable substrate holder, in order to obtain 8 different samples in a single deposition run. The deposition conditions were similar to those of the Nb/Pd multilayers described earlier

[13]. Two different sets of bilayers were prepared. They consist of a PdNi layer with constant thickness (dPdNiz500 A˚ ) and a

Nb layer with variable thickness (dNbZ150–1500 A˚ ). These

two series were used to determine TC(dNb) behaviour and to

estimate the Nb critical thickness. The superconducting transition temperatures TC were resistively measured using a

standard dc four-probe technique. The superconducting

Journal of Physics and Chemistry of Solids 67 (2006) 412–415

www.elsevier.com/locate/jpcs

0022-3697/$ - see front matter q 2005 Elsevier Ltd. All rights reserved. doi:10.1016/j.jpcs.2005.10.015

* Corresponding author. Tel.: C39 89 965 256; fax: C39 89 965 275. E-mail address: carla@sa.infn.it (C. Cirillo).

1

State University of Computer Science and RadioElectronics, P. Brovka street 6, 220600 Minsk, Belarus

transition temperature was defined as the midpoint of the transition curve.

The measured values of the Nb and PdNi resistivities on samples deliberately fabricated, 2000 and 300 A˚ thick, were, respectively, rNbZ6 mU cm and rPdNiZ24 mU cm. The Nb

critical temperature was TCZ9 K. Thus, the Nb coherence

length was also determined through the dirty limit expression: xSZ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃZDNb=2pKBTC

p

. Here, DNb is the diffusion coefficient

which is related to the low temperature resistivity rNbthrough

the electronic mean free path lNbby DNbZ vFNblNb=3, in which

lNbZ ð1=vFNbgNbrNbÞðpkB=eÞ2 [14], where gNbz7 !102J=K2

m3 is the Nb electronic specific heat coefficient [15] and
vF_{Nb}Z 2:73 !107cm/s is the Nb Fermi velocity [16]. We
obtained xNbz83 A˚ .

In the study of proximity effect, the control of interfaces properties is essential. For this reasons interface quality have been studied by X-ray reflectivity measurements, using a Philips X-Pert MRD high-resolution diffractometer. X-ray reflectivity analysis have been performed on bilayers deliber-ately fabricated with the appropriate thicknesses in the same conditions of the samples used in superconductivity measure-ments. The reflectivity profile of a Nb/PdNi bilayer with dNbZ

180 and dpdNiZ237 A˚ is shown in Fig. 1 together with the simulation curve obtained using the Parrat and Nevot-Croce formalism[17,18]. The fit gives a roughness value of 12 A˚ . The film thicknesses obtained from the simulation were used for the final calibration of dNband dpdNi.

The onset of ferromagnetism in Pd1KxNixalloys is around

xZ0.23[19]. In order to have a magnetic homogeneity a Pd1K xNixtarget with xZ10% was used: This stoichiometry was not

conserved in the samples as revealed by Rutherford Back-scattering Spectrometry analysis, which gives a Ni concen-tration of xZ0.14. For Pd90Ni10 alloys the value of the

exchange energy was estimated by saturation magnetization measurements, EexZ15 meV [2]. Using the values of the

measured low temperature resistivity rPdNiand of the Pd Fermi

velocity vF_{Pd}Z 2 !105cmsK1 _{[20]}_{, knowing the product}

rPdlPdZ4!10K5mU cm2 [21], we evaluated the diffusion
coefficient D_{PdNi}_{Z v}F

PdlPd=3, resulting in xFz60 A˚ .

It is well known that in metals electronic transport properties are closely related to magnetic ones. In particular electrical resistance measurements can give useful indications on the onset of magnetic ordering in metallic systems. For this reason we studied the critical behaviour of the electrical resistance of single PdNi films and of Nb/PdNi bilayers in the temperature range in which the magnetic ordering changes. From this measurements it is possible to estimate the Curie temperature of the alloy[24–26]. InFig. 2a, the behaviour of the normalized electrical resistance, R(T)R10 K, of a series of

Nb/PdNi bilayers is reported in the temperature range between 125 and 250 K. At high temperature, it is linear in T, but a broad maximum is present at Tz185 K, which become more and more evanescent as the Nb thickness is increased. But is the singular behaviour of R(T) first derivative, which better characterize the transition. In Fig. 2b, the temperature dependence of r(T)ZR(T)KR5 K and of dr/dT is presented

for the Nb/PdNi bilayer with dNbZ200 A˚ : the lowest

temperature at which the derivative shows a maximum can be taken as TCurie[22–24]. In this case, the magnetic transition

temperature can be approximately estimated as TCuriez156 K,

indicating that in the temperature range investigated for the superconducting measurements, the magnetic ordering is well established. The value obtained for the magnetic transition seems to be lower than the one derived by extraordinary Hall effect measurements [21]. Similar discrepancies have already been reported for other magnetic systems when TCurieobtained

by resistivity measurements is compared with the one obtained by saturation magnetization measurements[24].

3. Experimental results

The dependence of the critical temperatures TC on dNbof

Nb/PdNi bilayers is reported in Fig. 3. The transition temperature of the sample with dNbZ150 A˚ is not reported

since it was below 2 K, the lowest temperature reachable with our experimental setup. From this curve, we can extract dcr

NbZ 145 A˚ the minimum Nb layer thickness needed for

superconductivity to develop. Comparing this result with the
one obtained for Nb/Pd trilayers[11,12], and keeping in mind
that the critical thickness of the bilayers is half of the
corresponding trilayers, an higher value of d_{Nb}cr is found,
indicating the stronger effect of the ferromagnet. This value is
lower than the ones reported for traditional S/F systems[9,27],
but higher than the one obtained for Nb/Cu1KxNixtrilayers[4],

where Cu1KxNixis another weak ferromagnet. This result may

be due both to the weak ferromagnetism of the alloy and probably also to the good transparency of the Nb/PdNi interface. Also the ratio between the critical thickness and the Nb coherence length can be calculated, giving dcrNb=xNbZ 1:75, corresponding to 3.5 for the trilayers case. It

depends both on interface transparency T [28], and on the strength of the pairing, lowering with increasing xF and

decreasing _{T. In S/F systems with TZ 1, d}scr=xs has its

theoretical upper limit close to 6[28]. However, in classical S/

Fig. 1. Experimental (solid line) and calculated (dashed line) low-angle reflectivity profile for a Nb/PdNi bilayer. The numerical simulation is arbitrarily shifted downward for sake of clearness.

F systems xSis an order of magnitude larger than xFand in this

limit the d_{S}cr=xS ratio is practically independent fromT[28].

Also for this reason, the study of S/F interface seems to be more interesting in the case of weak ferromagnet, having a larger value for the ferromagnetic coherence length.

In summary, we studied the transport properties of Nb/Pd86Ni14 bilayers grown by sputtering. In particular the attention was devoted to the dependence of the superconduct-ing transition temperature on the thickness of the Nb layer with the thickness of the PdNi layer fixed at 500 A˚ . As main conclusion we deduced the superconducting critical thickness, dScr~145 A˚ . This value is lower than the ones reported for traditional S/F systems (because of the weak ferromagnetism of the alloy), but higher than the one obtined for Nb/Cul-xNix trilayers, with xZ0.67, 0.59 and 0.52. Further studies on this system are still in progress, as the fabrication of bilayers with PdNi variables thickness which could give an estimation of the ferromagnetic coherence length and could eventually reveal an oscillatory behaviour of the superconducting critical

.

Fig. 2. (a) Normalized electrical resistence, R(T)/R10 K, of a series of Nb/PdNi bilayers. (b) Rescaled resistance r(T)ZR(T)KR5 K(open symbols) compared with its first derivative (solid symbols) for the Nb/PdNi bilayer with dNbZ200 A˚ . The arrow indicates the value of TCurie.

Fig. 3. Critical temperature TCversus Nb thickness dNb. Different symbols refer to samples sets obtained in different deposition runs. The solid line is meant to guide the eye. The arrow indicates the value of dcr

Nb.

C. Cirillo et al. / Journal of Physics and Chemistry of Solids 67 (2006) 412–415 414

temperature. Moreover the interpretation of these results in the framework of recent theoretical model [7] could allow an evaluation of the interface transparency of the system. References

[1] J.S. Jiang, D. Davidovic, Daniel H. Reich, C.L. Chien, Phys. Rev. Lett. 74 (1995) 314.

[2] T. Kontos, M. Aprili, J. Lesueur, X. Grison, Phys. Rev. Lett. 86 (2001) 304. [3] V.V. Ryazanov, V.A. Oboznov, A. Yu. Rusanov, A.V. Veretennikov,

A.A. Golubov, J. Aarts, Phys. Rev. Lett. 86 (2001) 2427.

[4] A. Rusanov, R. Boogaard, M. Hesselberth, H. Sellier, J. Aarts, Physica C 369 (2002) 300.

[5] E.A. Demler, G.B. Arnold, M.R. Beasley, Phys. Rev. B 55 (1997) 15174. [6] Z. Radovic, M. Ledvij, L. Dubrosavljevic-Grujic, A.I. Buzdin, J.R. Clem,

Phys. Rev. B 44 (1991) 759.

[7] Ya.V. Fominov, N.M. Chtchelkatchev, A.A. Golubov, Phys. Rev. B 66 (2002) 14507.

[8] L.R. Tagirov, Physica C 307 (1998) 145.

[9] Th. Mu¨hge, K. Westerholt, H. Zabel, N.N. Garif’yanov, Yu.V. Goryunov, I.A. Garifullin, G.G. Khaliullin, Phys. Rev. B 55 (1997) 8945. [10] Th. Mu¨hge, N.N. Garif’yanov, Yu.V. Goryunov, G.G. Khaliullin,

L.R. Tagirov, K. Westerholt, I.A. Garifullin, H. Zabel, Phys. Rev. Lett. 77 (1996) 1857.

[11] M. Ve´lez, M.C. Cyrille, S. Kine, J.L. Vincent, I.K. Schuller, Phys. Rev. B 59 (1999) 14659.

[12] C. Cirillo, S.L. Prischepa, M. Salvato, C. Attanasio, Eur. Phys. J. B38 (2004) 59.

[13] C. Cirillo, S.L. Prischepa, A. Romano, M. Salvato, C. Attanasio, Physica C 404 (2004) 95.

[14] C. Cirillo, C. Attanasio, L. Maritato, L.V. Mercaldo, S.L. Prischepa, M. Salvato, J. Low Temp. Phys. 130 (2003) 509.

[15] P.R. Broussard, Phys. Rev. B 43 (1991) 2783.

[16] Handbook of Chemistry and Physics, in: R.C. Weast (Ed.), The Chemical Rubber Co., Cleveland, 1972.

[17] H.R. Kerchner, D.K. Christen, S.T. Sekula, Phys. Rev. B 24 (1981) 1200. [18] E.E. Fullerton, I.K. Schuller, H. Vanderstraeten, Y. Bruynseraede, Phys.

Rev. B 45 (1992) 9292.

[19] L.G. Parrat, Phys. Rev. B 95 (1954) 359.

[20] L. Nevot, P. Croce, Rev. Phys. Appl. 15 (1980) 761. [21] A. Tari, B.R. Coles, J. Phys. F Met. Phys. 1 (1971) L69.

[22] L. Dumoulin, P. Nedellec, P.M. Chaikin, Phys. Rev. Lett. 47 (1981) 208.

[23] T. Kontos, PhD Thesis, Universite´ Paris XI Orsay, 2002.

[24] M.P. Kawatra, S. Skalski, J.A. Mydosh, J.I. Budnick, Phys. Rev. Lett. 23 (1969) 83.

[25] M.P. Kawatra, J.I. Budnick, J.A. Mydosh, Phys. Rev. B 2 (1970) 1587. [26] J.A. Mydosh, J.I. Budnick, M.P. Kawatra, S. Skalski, Phys. Rev. Lett. 21

(1968) 1346.

[27] L. Lazar, K. Westerholt, H. Zabel, L.R. Tagirov, Yu.V. Goryunov, N.N. Garif’yanov, I.A. Garifullin, Phys. Rev. B 61 (2000) 3711. [28] J. Aarts, J.M.E. Geers, E. Bru¨ck, A.A. Golubov, R. Coehoorn, Phys. Rev.

B 56 (1997) 2779.